OPEN

Received: 18 October 2016 Accepted: 4 April 2017 Published: xx xx xxxx

Spin-orbit-torque-induced magnetic domain wall motion in Ta/CoFe nanowires with sloped perpendicular magnetic anisotropy Yue Zhang1,2, Shijiang Luo1, Xiaofei Yang1 & Chang Yang3 In materials with the gradient of magnetic anisotropy, spin-orbit-torque-induced magnetization behaviour has attracted attention because of its intriguing scientific principle and potential application. Most of the magnetization behaviours microscopically originate from magnetic domain wall motion, which can be precisely depicted using the standard cooperative coordinate method (CCM). However, the domain wall motion in materials with the gradient of magnetic anisotropy using the CCM remains lack of investigation. In this paper, by adopting CCM, we established a set of equations to quantitatively depict the spin-orbit-torque-induced motion of domain walls in a Ta/CoFe nanotrack with weak Dzyaloshinskii–Moriya interaction and magnetic anisotropy gradient. The equations were solved numerically, and the solutions are similar to those of a micromagnetic simulation. The results indicate that the enhanced anisotropy along the track acts as a barrier to inhibit the motion of the domain wall. In contrast, the domain wall can be pushed to move in a direction with reduced anisotropy, with the velocity being accelerated by more than twice compared with that for the constant anisotropy case. This substantial velocity manipulation by anisotropy engineering is important in designing novel magnetic information devices with high reading speeds. Since the concept of “race-track storage” was proposed in 20081, current-induced magnetic domain wall motion in nanotracks has attracted wide research interest because of its application potential in next-generation memory-storage devices with advantages such as low dissipation, high reading speed, small size, and large storage density. The basic physical principle underlying such devices is the exchange of angular momentum between the spins of conducting electrons and magnetic moments in the domain wall due to the spin-transfer torque (STT) or spin-orbit torque (SOT). Recently, SOT-driven domain wall motion has attracted wide attention because of its high energy efficiency2–4. Unlike the bulk STT in a single ferromagnetic nanotrack, the SOT dominates in multilayer films, such as heavy metal (HM)/ferromagnet (FM) multilayer2, 3, 5 or HM/FM/oxide multilayer with broken inversion symmetry at the interface4. The SOT effect in the multilayer system can originate from the spin Hall effect (SHE) of the HM layer. Recently, some intriguing SOT-induced magnetization behaviours have been discovered in HM/FM bi-layers with sloped magnetic parameters. For example, Yu et al. discovered field-free magnetization switching in a Ta/CoFeB perpendicularly magnetized (PM) film with magnetic anisotropy gradient6. They attributed this phenomenon to an effective magnetic field originating from the gradient of the magnetic anisotropy constant. From a microscopic perspective, the SOT-induced magnetizing process in a HM/FM multilayer is generally related to the motion of the FM domain wall. For example, the domain wall exhibits chirality and an unexpected Néel-typed structure in the HM/FM multilayer with interfacial Dzyaloshinskii–Moriya interaction (DMI)3, 7. The direction of the motion of the domain wall is also related to the sign of the DMI constant and to that of the spin Hall angle of the HM4, 8–10. In addition, the domain wall also tilts because of strong DMI, which has been experimentally observed11, 12 and theoretically proven9, 13–16. Additionally, domain wall motion is closely linked to the

1

School of Optical and Electronic Information, Huazhong University of Science and Technology, Wuhan, 430074, PR China. 2Department of Physics and Astronomy, Johns Hopkins University, Baltimore, MD, 21218, USA. 3Department of Mathematics, Harbin Institute of Technology, Harbin, 150001, PR China. Correspondence and requests for materials should be addressed to C.Y. (email: [email protected])

Scientific Reports | 7: 2047 | DOI:10.1038/s41598-017-02208-y

1

www.nature.com/scientificreports/

Figure 1. Schematic of SOT-driven domain wall in a nanotrack with magnetic anisotropy gradient. (The theoretic analysis in the paper is based on the up-down domain wall structure in the coordinate system shown in Fig. 1). magnetic anisotropy constant which can be controlled effectively by manipulating the thickness of the film or by being situated in an electric field17–20. Despite recent progress, determining how the domain wall moves in a HM/FM multilayer with the gradient of magnetic anisotropy remains to be elucidated. Yamada et al. proposed an effective field induced by the gradient of magnetic anisotropy and believe that this effective field can drive the wall to move21. However, the domain-wall motion in a magnetic system with anisotropy gradient has not been investigated using standard cooperative coordinate method (CCM), which is the basic route to quantitatively study the domain wall motion7, 22. In the present work, using CCM, we have deduced the equations to describe the SOT-driven domain wall motion in a HM/FM multilayer with the gradient of magnetic anisotropy and weak DMI. The equations were solved numerically and compared with the results of a micro-magnetic simulation. Based on the derived equations, the effect of magnetic anisotropy gradient on the domain wall motion has been revealed.

Principle and Methods

Numerical Calculation based on collective coordinate model. To quantitatively describe the dynamics of SOT-driven domain wall motion in a nanotrack with magnetic anisotropy gradient, we develop a one-dimensional (1D) CCM, where the DW is depicted by two collective coordinates: its central position q and the azimuthal angle ϕ of the DW magnetization in spherical coordinates, as shown in Fig. 1. Due to the weak DMI, the tilting angle of DW is not taken into consideration here9. The normalized vector for the direction of magnetization is described as → m = (sin θ cos ϕ, sin θ sin ϕ, cos θ). The polar angle θ and the azimuthal angle ϕ marked in Fig. 1 are included in the ansatz for the DW magnetization: θ = 2arctan{exp[(x − q)/∆]}, and ϕ = ϕ(t )

(1)

where t is the time, and ∆=

A /(K − µ 0MS2/2) ,

(2)

represents the width of the domain wall and A, μ0, MS, and K are the exchange stiffness constant, vacuum permeability, saturation magnetization, and magnetic anisotropy constant for the PMA film, respectively. In the present work, K = ax + b. This linear function K(x) is the simplest form for numerical calculation. From the aspect of experiments, to generate PM film with linearly varied K, one can fabricate PM film with a gradient of thickness along the track6 or by poling piezoelectric substrate in a wedge shape21. To determine the parameters a and b in the function K(x), one can pattern the sample into an array of Hall bar and fit the K-x relationship composed by the K data collected at different sites (x) using extraordinary Hall effect measurement6. The variation of magnetic anisotropy in the track may lead to a space-coordinate dependent ϕ. However, the width of the domain wall is comparatively smaller than the length of the entire track, and the magnetic anisotropy can remain to be considered constant in the region of the domain wall. Therefore, ϕ is also approximately invariant in the range of the domain wall. The Thiele equation for the domain wall motion is deduced by the Lagrangian approach. Let l be the Lagrangian density function and the expression can be written as follows13 l = E + (MS/γ )ϕθ sin θ ,

(3)

where γ is the gyromagnetic ratio, θ is the time derivative of θ, and E represents the total free energy density and can be written as E = Ee + Ea + Ed + E DM.

(4)

Ee, Ea, Ed, and EDM are the exchange energy density, magnetic anisotropy energy density, demagnetization energy density, and free energy density from DMI, respectively. They are written as Scientific Reports | 7: 2047 | DOI:10.1038/s41598-017-02208-y

2

www.nature.com/scientificreports/

Ee = A

∑

i=x ,y ,z

∇mi 2 ,

(5)

where ∇ is the Nabla symbol. 1 Ea = K − µ0MS2sin2θ , 2 Ed =

(6)

1 µ NxMS2sin2θ cos2ϕ, 2 0

(7)

E DM = D[mz(∂m x /∂x ) − m x (∂mz /∂z )],

(8)

and the demagnetization factor Nx is described by refs 9, 23 Nx = L z ln2/π ∆ ,

(9)

where Lz is the thickness of Co layer. For a non-conservative system, another dissipation density function fd should be included to depict the dissipation13: 2 →/dt − (γ /α)H (→ fd = (αMS/2γ)[dm 0 SO m × e y )] ,

(10)

where α is the damping coefficient, and HSO is the effective magnetic field due to SOT and is written as HSO = µ BθSHJ /γ0eMSL z,

(11)

where μB, θSH, J, and e are the Bohr magneton, spin Hall angle of the HM layer, current density, and charge of an electron, respectively. The parameter γ0 is related to γ by γ0 = μ0|γ|. The Lagrangian (L) and Rayleigh dissipation function (F) were determined by integrating l and fd with respect to the entire space region for the track. The Thiele equations are finally deduced using the Lagrange–Rayleigh equation: ∂L d ∂L ∂F − = 0, + ∂qi dt ∂q i ∂q i

(12)

where qi represents the collective coordinate q or ϕ and t is time. The domain wall motion in the track with magnetic anisotropy gradient is depicted by the following Thiele equations: (αMSI5/γ )q + (MSI8/γ A )ϕ = −A(∂I1/∂q) − a(∂I2/∂q) 1 − b − µ0MS2(∂I3/∂q) 2 − D cos ϕ(∂I4/∂q)

− (µ0L zMS2 cos2 ϕ ln2/2π A )

× (∂I8/∂q) − (MSγ0/γ )HSOI7 cos ϕ,

(13)

( −MSI8/γ A )q + (αMSI3/γ )ϕ = DI4 sin ϕ + (µ0L zMS2(ln2) × cos ϕ sin ϕ/π A )I8 + (MSγ0/γ )HSOI6 sin ϕ,

(14)

where I1–I8 are the integrals with the following formulas: I1 =

Lx 2

2

Lx 2

2

∂f

Lx 2

2

2

∫− L2x (sin θ) ∂x dx; I2 = ∫− L2x x(sin θ)dx; I3 = ∫− L2x sin θ dx; Lx 2 − Lx 2 Lx 2 − Lx 2

Lx 2 − Lx 2

I4 =

∫

∂f sin θ dx ; I5 ∂x

I7 =

∫

∂f sin θ dx ; I = 8 ∂q

∫

2

∂f (sin2 θ) dx ; I6 = ∂q Lx 2

∫− L2x

ax + b −

Lx 2 − Lx 2

∫

sin θ cos θ dx ;

1 µ MS2 (sin2 θ) dx . 2 0

(15)

Here, Lx is the length of nanotrack, and

Scientific Reports | 7: 2047 | DOI:10.1038/s41598-017-02208-y

3

www.nature.com/scientificreports/

f = (x − q) ax + b − sin θ =

2 exp(f ) ; 1 + [exp(f )]2

cos θ =

1 − [exp(f )]2 . 1 + [exp(f )]2

1 µ MS2 / A ; 2 0

(16)

Equations (14) and (15) were solved using a 4th-order Runge–Kutta algorithm with a time step of 1 ps. The integrals I1–I8 were numerically evaluated using an adaptive Gauss–Kronrod quadrature. In the calculation, the nanotrack has the dimensions 1 μm (length) × 100 nm (width) × 0.6 nm (thickness). Typical magnetic parameters for PM Ta/CoFe bilayers were used9:MS, b, A, D, and α for CoFe are 7 × 105 A/m, 4.8 × 105 J/m3, 1 × 10−11 J/m, −0.05 mJ/m2, and 0.03, respectively. The spin-Hall angle (θSH) for Ta is −0.11. The slopes for the anisotropy constant (a) are 0, 1 × 1011, 2 × 1011, and 3 × 1011 J/m4. A larger a cannot ensure effective perpendicular magnetic anisotropy throughout the entire track.

Micro-magnetic simulation. The motion of the domain wall in the nanotrack with magnetic anisotropy gradient was also investigated by micro-magnetic simulation using the software “object-oriented micromagnetic framework” (OOMMF) with code including DMI24. The principle of the simulation is based on solving the Gilbert equation → ∂→ ∂→ m m = −γ0→ m × Heff + α(→ m × ) + γ0HSO(→ m × (→ σ ×→ m )), ∂t ∂t

(17)

→ 1 δE Heff = − ( ), µ0MS δ→ m

(18)

→ where Heff is the effective magnetic field derived from the free energy density:

which includes the effective field from exchange, magnetic anisotropy, demagnetization, and DMI. We consider a Ta/CoFe nanotrack whose shape and magnetic parameters are identical to that in numerical calculation. In current OOMMF software, it is not possible to generate magnetic anisotropy constants that change with x continuously. As an approximation to the case of a = 3 × 1011 J/m4 and J = ±5 × 1011 A/m2 in numerical calculation, we fabricated an anisotropy constant that is a piecewise constant function of x. This piecewise constant function of K can be expressed as follows, 1 × 107 J/m3, ( − 500 nm, − 450 nm) K0, ( − 450 nm, ( − 450 + ∆x ) nm) K0 + ∆K , (( − 450 + ∆x ) nm, ( − 450 + 2∆x ) nm) K = K0 + 2∆K , (( − 450 + 2∆x ) nm, ( − 450 + 3∆x ) nm) K0 + N ∆K , (( − 450 + N ∆x ) nm, ( − 450 + (N + 1) ∆x ) nm) 1 × 107 J/m3, (450 nm, 500 nm) .

(19)

The anisotropy constant close to the two ending points of the track (from −500 to −450 nm and from 450 to 500 nm) was set as large as 1 × 107 J/m3 to pin boundary moments. The remaining nanotrack (x = −450 nm to x = 450 nm) was evenly divided into N + 1 steps with the size of Δx for every step. The anisotropy constant varies from 3.45 × 105 to 6.0 × 105 J/m3 in accordance with an even step of ΔK. In our simulation, N includes 35, 17, and 9. Accordingly, Δx includes 25 nm, 50 nm, and 100 nm, and ΔK includes 0.075 J/m3, 0.15 J/m3, and 0.3 J/m3, respectively.

Results

Figure 2 shows the current-induced evolution of the central position of the domain wall in the nanotrack with magnetic anisotropy gradient. The negative (positive) current induces the motion of the domain wall towards the positive (negative) x direction, and this indicates that the domain wall moves along the direction of the moving election but against that of the current. This direction is consistent with that for negative D and negative θSH4, 9. When a = 0 J/m4, a linear t–q relationship is well satisfied except at the initial moving stage (t